Polymer-based flexible Bioelectronic device abstract Due to the mechanical mismatch between...
Embed Size (px)
Transcript of Polymer-based flexible Bioelectronic device abstract Due to the mechanical mismatch between...
Science Bulletin 64 (2019) 634–640
Contents lists available at ScienceDirect
journal homepage: www.elsevier .com/locate /sc ib
Polymer-based flexible bioelectronics
Xiaoying Wu, Huisheng Peng ⇑ State Key Laboratory of Molecular Engineering of Polymers, Department of Macromolecular Science, and Laboratory of Advanced Materials, Fudan University, Shanghai 200438, China
a r t i c l e i n f o a b s t r a c t
Article history: Received 2 March 2019 Received in revised form 17 March 2019 Accepted 18 March 2019 Available online 5 April 2019
Keywords: Polymer Flexible Stretchable Multi-functional Bioelectronic device
https://doi.org/10.1016/j.scib.2019.04.011 2095-9273/� 2019 Science China Press. Published by
⇑ Corresponding author. E-mail address: firstname.lastname@example.org (H. Peng).
Due to the mechanical mismatch between conventional rigid electronic devices and soft tissues at nature, a lot of interests have been attracted to develop flexible bioelectronics that work well both in vitro and in vivo. To this end, polymers that can be used for both key components and substrates are indispensable to achieve high performances such as high sensitivity and long-term stability for sensing applications. Here we will summarize the recent advances on the synthesis of a variety of polymers, the design of typ- ical architectures and the integration of different functions for the flexible bioelectronic devices. The remaining challenges and promising directions are highlighted to provide inspirations for the future study on the emerging flexible bioelectronics at end.
� 2019 Science China Press. Published by Elsevier B.V. and Science China Press. All rights reserved.
With the rapid development on cooperation studies among materials science [1,2], electronic engineering, artificial intelli- gence, and biomedical science, there emerges a new and multidis- ciplinary direction which is named bioelectronics [3–9]. In most cases, it represents the design and application of electronic devices such as sensors to solve the problems of biomedical fields, includ- ing both in vitro and in vivo. Obviously, the conventional rigid elec- tronic devices typically based on metal and silicon electrodes cannot effectively meet the requirements of soft tissues mainly in mechanical property such as stiffness. If a rigid device is attached to the skin or implanted into the body, the surrounding tissues may get hurt and the resulting scars will damage or even disable the devices . Out of question, it is well expected that bioelectronic devices should mechanically behave like the soft tis- sue after being adhered to or implanted. They should be also bio- compatible and stable upon contact with biofluids to avoid the coating failure, delamination or corrosion . In the case of their applications in vivo, they would not be peeled off or extracted from the body to avoid second injury after use. In other words, they would better degrade in body or be assimilated/metabolized by the body . In addition, an ideal electronic device should be implanted with minimal traumas  (e.g., by injection through the use of a needle) and may accommodate body movements (e.g., it is able to bear stretching, compressing, folding or other deformations) . Furthermore, it is better to easily integrate
Elsevier B.V. and Science China Pr
the other functions such as powering and data transferring in the bioelectronic devices with small sizes [3,15,16], which are vital to the applications both in vitro and in vivo.
To fully satisfy the biomedical applications, increasing interests have been thus attracted to develop the next-generation flexible electronic devices with a variety of functions in recent years. They can be soft, deformable, stable, biocompatible and even degradable to open up a new avenue in the advance of detecting signals or dis- eases, understanding mechanisms of biological activities, treating diseases and communicating . The effective applications are mainly derived from the good and dynamically matching interfaces [6,16]. For the use of a flexible device in vitro, it can closely attach on curved skin surface with a stable interface and thus works effi- ciently under moving [18–20]. In the case of the flexible device in vivo, the stable and dynamically matching interfaces between the flexible electronic device and tissues are also found to play a critical role in high biocompatibility [21–23]; In contrast, the stiff implants induce astrocytic scars and microglia populations (Fig. 1).
The effective interfaces are closely related to the use of soft materials for key components or/and substrates, the design of structures and the realization of functions in flexible bioelectronic devices . Polymers are first highlighted due to the fact that they have been typically explored as the promising soft materials, in addition to the basis of the structure and property design. The rep- resentative structures and properties are then summarized for the available flexible electronic devices. The remaining challenges and promising directions are finally presented to give an inspiration to the future study in flexible bioelectronics.
ess. All rights reserved.
https://doi.org/10.1016/j.scib.2019.04.011 mailto:email@example.com https://doi.org/10.1016/j.scib.2019.04.011 http://www.sciencedirect.com/science/journal/20959273 http://www.elsevier.com/locate/scib
Fig. 1. (Color online) Interface demands for implantable bioelectronics. A schematic comparison on the foreign body response of stiff (top) and compliant (bottom) bioelectronic devices. Reprinted with permission from Ref. , Copyright 2017 Nature Publishing Group.
X. Wu, H. Peng / Science Bulletin 64 (2019) 634–640 635
2. Polymer materials
The diversity and synthetic tunability of polymer materials offer them good electrical conductivity for electrodes, optical trans- parency for substrates and biodegradability for sacrificial layers in bioelectronic devices  (Fig. 2a). Polyaniline (PANI), poly(3,4 -ethylenedioxythiophene) (PEDOT) and polypyrrole (PPy) are widely used as electrodes [1,25,26]. Generally, if organic com- pounds including high boiling solvents like dimethyl sulfoxide and methyl pyrrolidone, ionic liquids and surfactants are added, their electrical conductivities may increase to be comparable to indium tin oxide (ITO), a typical inorganic electrode material. Silk, cellulose, collagen, gelatine and other natural polymers with both high biocompatibility and biodegradation are good candidates for sacrificial layers that can degrade and dissolve after implanting, thus minimizing the invasion for better recording or stimulation [27–29]. Meanwhile, synthetic polymers such as polylactic acid, polyethylene glycol and their copolymers are also competitive alternatives as sacrificial layers due to their tuneable degradation rates and good biocompatibility . As moisture and dielectric bar- riers, polymers like polydimethylsiloxane (PDMS), poly(p- xylylene) (mostly used as a trade name of Parylene C), and poly- imide (PI) are widely explored as insulation substrates to protect electric components from impairing under direct contacts with biofluids [5,27,30]. These polymers are transparent, flexible and biocompatible without immune responses. Note that polymers are advantageous for large-scale and low-cost preparations through solution processes such as spin coating .
Metal and silicon can be in fact made into nanomaterials to realize flexibility on the device level, though they cannot change their intrinsic rigid property, e.g., high elastic modulus of �100 GPa for silicon. In contrast, polymers show much lower and tune- able elastic moduli ranged from 100 kPa to 10 GPa, which may be designed to match biological tissues (typically 1 kPa to 1 GPa for soft tissues and 10 GPa for hard tissues) to great degree [6,32,33] (Fig. 2b). Compared with silicon, the use of inherently soft polymer materials to directly contact biological tissues may greatly reduce negative reactions for bioelectronic devices owing to the better interfaces between the devices and tissues.
To prevent the failure of bioelectronic devices, it is also neces- sary to seal them from exposure to warm, aqueous and saline envi- ronments associated with the foreign-body response mostly by the use of polymers. Polymers like PDMS and poly(p-xylylene) that are commonly explored for clinical applications have been widely investigated as effective sealing layers. If cracks still occur, we may introduce self-healing polymers in advance to bioelectronic devices and restore them with high stability [20,34,35] (Fig. 2c).
3. Structure designs
For human skins, organs and brain skulls with curved surfaces, it is challenging for typical thin-film bioelectronic devices to attach to them seamlessly, which for instance results in acute stimulation or inaccurate detection. Consequently, hydrogels and adhesive polymers may be used to improve compliant contacts by increasing the adhesion force between devices and tissues [3,23].
Fig. 2. (Color online) Polymers for soft interface and functionalization. (a) Different components with different polymers of a flexible bioelectronic device. (b) Logarithmic plot on the comparison of elastic moduli for various biological tissues and materials. (c) The realization of self-healing function by the use of self-healing polymer. Reprinted with permission from Refs.  and , Copyright 2017 Nature Publishing Group and 2013 Wiley-VCH Verlag.
636 X. Wu, H. Peng / Science Bulletin 64 (2019) 634–640
A representative strategy is to modify the structure of the bioelec- tron